Post on 27-Nov-2014
Embed Size (px)
High-Performance Alloys for Resistance to Aqueous CorrosionWrought nickel productsThe INCONEL Ni-Cr, Ni-Cr-Fe & Ni-Cr-Mo Alloys The INCOLOY Fe-Ni-Cr Alloys The MONEL Ni-Cu Alloys
ContentsCorrosion Problems and Alloy Solutions Corrosion-Resistant Alloys from the Special Metals Group of Companies Alloy Selection for Corrosive Environments Corrosion by Acids Sulfuric Acid Hydrochloric Acid Hydrofluoric Acid Phosphoric Acid Nitric Acid Organic Acids Corrosion by Alkalies Corrosion by Salts Atmospheric Corrosion Corrosion by Waters Fresh and Process Waters Seawater and Marine Environments Corrosion by Halogens and Halogen Compounds Fluorine and Hydrogen Fluoride Chlorine at Ambient Temperature Chlorine and Hydrogen Chloride at High Temperatures Metallurgical Considerations Appendix 1
11 12 12 17 20 22 25 26 28 31 35 37 37 38
40 40 41 41 44 49
Corrosion Science and Electrochemistry 50 References 60
Publication number SMC-026 Copyright Special Metals Corporation, 2000 INCONEL, INCOLOY, MONEL, INCO-WELD, DURANICKEL, 625LCF, 686CPT, 725, 864 and 925 are trademarks of the Special Metals group of companies.
Special Metals Corporation
Corrosion Problems and Alloy SolutionsDue to their excellent corrosion resistance and good mechanical properties, the Special Metals nickel-based alloys are used for a broad range of applications in an equally broad range of industries, including chemical and petrochemical processing, pollution control, oil and gas extraction, marine engineering, power generation, and pulp and paper manufacture. The alloys' versatility and reliability make them the prime materials of choice for construction of process vessels, piping systems, pumps, valves and many other applications designed for service in aqueous and high-temperature environments. Many variables influence the performance of a specific material in a specific environment. These include concentration, temperature, aeration, liquid or gaseous flow rates, impurities, abrasives, and cycling process conditions. While every attempt has been made to present a broad base of information, more detailed data will often be needed for individual applications and environments. The reader is encouraged to contact Special Metals marketing and technical staff for more specific alloy properties and a wealth of experience of applications and alloy service and performance.
Corrosion problems can be found in many forms.Metallic corrosion under aqueous conditions can take place by many mechanisms with quite varied results. A brief general description of each type of corrosion is presented here as an introduction. More detail of the mechanics of the various types of corrosion is presented later in this publication under Corrosion Science and Electrochemistry.
Crevice Corrosion Crevice attack usually takes placein a very tight gap between two surfaces (e.g. as with gaskets or fasteners or under mineral deposits). As with pitting, the micro-environment within the crevice can greatly differ from the general medium. Concentration cells can cause this type of corrosion to progress at a very rapid rate. Microbially Influenced Corrosion (MIC) MIC is a recently identified form of crevice attack. Certain types of bacteria form dome-shaped colonies on the metallic surface. The inside of the structure is sealed from the outside. The life cycle of the bacteria produces a corrosive environment within the colony which causes a crevice attack of the metal. While MIC usually takes place on components exposed to natural water (either fresh or brackish), it has also been encountered in process water in industrial systems. Environmentally Assisted Cracking Some types of corrosion take place as a result of chemical conditions within the environment and the mechanical condition of the metal itself. Both conditions must be present for this type of corrosion to take place. Corrosion fatigue, stress corrosion cracking, liquid metal cracking, and hydrogen embrittlement are all forms of environmentally assisted cracking.
General Corrosion General corrosion is a uniform attack and is the most commonly encountered type of corrosion. It is characterized by a chemical or electrochemical reaction which proceeds uniformly over the entire exposed surface area. The metal becomes thinner and eventually fails. Localized Corrosion Conditions may exist that causecorrosive attack in a very specific location or under a specific set of conditions. Such attack is normally referred to as localized. This type of corrosion takes several forms. Pitting, crevice attack, and microbially influenced corrosion (MIC) are all types of localized corrosion.
Pitting Pitting is a form of very localized attack thatresults in the formation of holes in the metal. While the holes formed are generally small they can propagate very quickly leading to material perforation and failure in a very short period of time. The micro-environment within the pit itself can be autocatalytic making this a particularly dangerous form of attack.
Corrosion Fatigue Corrosion fatigue failure takesplace due to the reduction of fatigue resistance of the metal with the presence of a corrosive medium. Thus it is normally encountered not as a visible degradation of the metal but as a premature failure of a component under cyclic conditions. The stress under which the material fails would not normally be considered sufficient to cause failure.
Stress Corrosion Cracking This refers to the cracking caused by the simultaneous presence of tensile stress and a specific corrosive medium. During this type of cracking, the metal is virtually unattacked over most of the surface while fine cracks progress through it at the attack site. Chloride stress cracking of stainless steels and ammonia stress cracking of nickel-copper alloys are examples of this type of attack.
most reactive nature. Because of thermal mechanical processing, metallic compounds may tend to precipitate and migrate to the grain boundaries. If these are more reactive than the metallic matrix, they can be selectively attacked. Metallic reactions can cause areas adjacent to the grain boundary to be depleted of some element, rendering this zone less resistant to attack. A commonly encountered form of intergranular corrosion is the attack of non-stabilized austenitic stainless steels due to the formation of chromium carbide precipitates and the subsequent depletion of chromium.
Erosion Corrosion Erosion corrosion is the acceleration or increase in rate of deterioration or attack on a metal because of relative movement between a corrosive medium and the metal surface. Generally the movement is rapid and the effects of mechanical wear or abrasion are involved. Metal is removed from the surface as dissolved ions or corrosion products are mechanically swept away from the metal surface.
Liquid Metal Cracking Liquid metal cracking is aspecialized form of stress corrosion. The susceptible metal (usually due to residual tensile stresses from fabrication) is attacked (cracked) by a low-melting liquid metal. An example is the cracking of aged Ni-Cr-Fe alloys by silver-base braze alloys.
Galvanic Corrosion Galvanic corrosion results fromthe electrical coupling of two dissimilar metals in a corrosive medium resulting in the attack of the less resistant metal. The metallic differences may be due to metallic structure as well as composition. The less noble material becomes anodic while the more noble becomes cathodic. The anodic material actually protects the cathodic leading to its own accelerated decay. Ranking of materials in an electromotive force (EMF) or galvanic series in a specific media will help determine the propensity of two materials for this type of corrosion. The farther apart the materials are in the series, the greater is the likelihood of attack of the less noble material.
Hydrogen Embrittlement Hydrogen embrittlementtakes place due to the penetration of the surface of susceptible metals by elemental hydrogen. This can result from the formation of metallic hydride compounds in some materials while in others it takes place by the interaction of dissolved hydrogen atoms. Regardless of the mechanism, the attack results in the formation and propagation of fine cracks and voids in the metallic structure.
Intergranular Corrosion Intergranular corrosion,as the name implies, is the selective attack of a metallic component at the grain boundaries by a corrosive medium. Several conditions can lead to a material being susceptible to intergranular corrosion. In some environments the grain boundary of a metal simply exhibits the
Dealloying Dealloying (also referred to as selectiveleaching) is the selective removal of one element of a solid alloy by a corrosion process. A corrosive medium specifically attacks one component of the alloy. A common example of this type of corrosion is the selective removal of zinc from brass (dezincification).
The solutions to the problems can be found in nickel and its alloying elements.Nickel retains an austenitic, face-centered-cubic (fcc) crystal structure up to its melting point, providing freedom from ductile-to-brittle transitions and minimizing the fabrication problems that can be encountered with other metals. In the electrochemical series, nickel is more noble than iron but more active than copper. Thus, in reducing environments, nickel is more corrosion resistant than iron, but not as resistant as copper. Alloying with chromium provides resistance to oxidation thus providing a broad spectrum of alloys for optimum corrosion resistance in both reducing and oxidizing environments. Nickel-based alloys have a higher tolerance for alloying elements in solid solution than stainless steels and other iron-based alloys but main